SSI Failure Analysis Handbook
Embed Size (px)
Transcript of SSI Failure Analysis Handbook
- 1. Failure Analysis Guide Eliminate Potential and Future Problems
- 2. Applications Require High Performance Todays demanding applications require high- performance, leak-free seals. From agricultural equipment to injection molding machines, hydraulic seals are expected to function throughout their respective lifespan without failure. Although a relatively small expense in the overall price of a hydraulic cylinder, factors at stake from early failure are: Expense of Down Time Loss of Production Pollution Potential Danger to Humans Accurate failure analysis is a critical step in eliminating current and future problems.
- 3. Modes of Failure PAGE Abrasion 05 Extrusion 06 Dieseling 07 Explosive Decompression 08 Pressure Trapping 09 Contamination 10 Heat Damage 11 Swelling 12 Hydrolysis 13 Flex Fatigue/Fracture 14 Side Loads 15 Erosion 16 Dry Running 17 Over Pressurization 18 Other Factors 19 MAINTENANCE & REPAIR Interruptions. Are. Bad. For. Pro. Duc. Tiv. Ity. Interruptions in many operations can cost millions of dollars in lost productivity. Thats why System Seals maintains a 24-hour emergency response service, which fills orders and expedites delivery faster than any other supplier in the industry. Nights, weekends, holidayswhen seals fail, its really your profit margin thats leaking. This guide is intended to provide insight into why seals fail and factors that contribute to seal failure. Its a starting point that System Seals engineers use to engineer the next generation of seal systems that prevent failure, reduce downtime and save our customers a substantial amount of money in gained productivity. For more information about maximizing your seal performance, talk directly to an engineer today at 216.220.1800, or visit our web site at www.systemseals.com.
- 4. Abrasion Accelerated wear of the seal by outside influences. CONTRIBUTING FACTORS Surface finish thats too rough Damaged sliding surface Insufficient lubrication Contamination MACHINING RECOMMENDATIONS Rods that ground with non-oriented finish or roller burnishing Barrels honing and roller burnishing HARDNESS Heat treat to 45-60HRC to a minimum depth of 0.5mm. CORROSION PROTECTION Hard chrome overlay with coating thickness 30-50m. FINISH RE-WORK AFTER CHROME Super-finish or polish to obtain final surface finish recommendations. SURFACE FINISH RECOMMENDATIONS To maximize seal performance and durability, System Seals Inc. recommends the following finishing values for hydraulic seals. Surface Roughness Surface Finish Ra Rt RMS sliding surface 0.3m 3.0m 8 groove root 1.8m 10.0m 32 groove sides 3.0m 16.0m 125 Note: System Seals, Inc. recommends to not only rely on the above information, but to also measure the profile bearing area ratio Tp. Knowing the profile bearing area ratio will ensure a surface quality that is optimum for hydraulic seals. Recommendation: Tp should be between 50-90% of the average height value C=Rz/2 with reference line at Cref=0 Above: NBR piston u-cup with abrasion marks at the seal lip and migrating across the dynamic surface. Above: Close up view of a u-cup seal lip showing abrasion marks. Above: PTFE seal with abrasion marks at the seal lip and migrating across the dynamic surface. Not suitable for a sealing surface. Within recommendation for a good sealing surface. Tp=39% Tp=79% 06 07 systemseals.com
- 5. Dieseling Damage caused by air bubbles within the oil. The fumes within the bubbles ignite when pressurized, causing burning of the seal face. CONTRIBUTING FACTORS Unpurged air from oil prior to operation Rapid pressure rise Above: Polyurethane u-cup with dieseling damage. Above: Nylon back-up ring with dieseling damage. Above: Rapid pressure rise squeezes the air bubbles, causing immense heat which is hot enough to ignite the oil fumes trapped within the bubbles. The result is a burning of the seal face. EXTRUSION CORRECTIVE ACTION There is design criteria for extrusion gaps and this criteria is based on the seal material and operating pressures. However, situations arise where the recommendations cannot be met, such as cylinder re-build. To overcome the extrusion potential, seals using back-up rings or the use of reinforced materials are recommended. Back-up Ring Extrusion Gap 2.0 1.9 1.8 1.7 1.6 1.5 1.4 1.3 1.2 1.1 1.0 0.9 0.8 0.7 0.6 0.5 0.4 0.3 0.2 0.1 0.0 Above: V-packing female adapter ring showing clear signs of extrusion. Extrusion Damage to the seal from the gap between the sliding surface and housing. Excessive gaps allow the seal to deform into these gaps under pressure, causing material to creep and/or break off. CONTRIBUTING FACTORS System pressure too high Larger than normal extrusion gap Cylinder expansion Wrong seal material Above: Polyurethane static seal showing signs of extrusion. Above: PTFE piston seal showing signs of severe extrusion. Below: Seals shown are examples of the types of seal designs recommended should a customer have large clearances within their applications (large gap conditions). E-GAP(MM) PRESSURE (BAR) 0 100 230 300 400 500 Polyacetal at 230F at 3000 hours 600 650 700 2.0x1.5 2.5x2.0 3.5x2.5 5.0x3.5 7.5x5.0 P Above: Polyurethane u-cup showing severe dieseling damage. 08 09 systemseals.com
- 6. Above: Back-to-back piston u-cup seals showing pressure trapping with reverse extrusion as a result. Pressure Trapping Typical for piston applications using two seals, oil gets trapped between the seals during operation. This oil volume increases with time, creating pressure and eventually forcing the seals away from each other, causing damage. CONTRIBUTING FACTORS Incorrect seal design; ie. no pressure relieving ability Long stroke High speed Above: Loaded polyurethane u-cups showing severe pressure trapping and failure. Above: Normal action of piston can cause certain types of piston seals to trap pressure. Above: Excessive pressure between the seals can push the seals away from each other, ultimately resulting in pressure trapping failure. Above: Polyurethane u-cup seal damaged by explosive decompression. Explosive Decompression Damage caused by gas permeating within the seal material under pressure. The gas, in the form of a collapsed bubble, expands when pressure drops, resulting in blistered seal material. CONTRIBUTING FACTORS Incompatible seal material High pressure High temperature Long exposure time of seal material to media under pressure Above: Damaged by explosive decompression. Above: Polyurethane u-cup seal damaged by explosive decompression. 010 011 systemseals.com
- 7. Above: Polyurethane u-cup seal with severe heat damage/cracking. Heat Damage Damage to the seal from excessive temperatures. The result is a hardening of the elastomer, which can cause permanent deformation, discoloration, cracking and material breaking off. CONTRIBUTING FACTORS High speed operation, which affects the seal lip Hot oil or environment, exposing the whole seal to high temperatures Incorrect seal material Above: Inner lip of a nitrile rotary shaft seal that has cracked from high running temperatures. Above: Polyurethane u-cup seal with severe heat damage/cracking. Above: Multi-component piston seal exposed to temperatures that caused the components to melt. Contamination Damage to the sealing components from solid particles during operation. CONTRIBUTING FACTORS Dirty assembly area Internal cylinder contamination; ie. cylinder wear over time causing clogged filters, dirty oil, metal particles Poor wiper performance Above: Hydraulic cylinder with severe contamination. Above: Hydraulic cylinder operating in a severe salt contaminated environment. Above: Resin/Fabric guide band damaged by severe metallic contamination. 012 013 systemseals.com
- 8. Above: Polyurethane o-ring showing early signs of hydrolysis. Hydrolysis Break-down of the seal material from exposure to water or water based fluids at elevated temperatures. The result is a loss of physical properties, cracking and crumbling of the material. CONTRIBUTING FACTORS Incompatible seal material for fluid used High temperatures Above: Thermoplastic elastomer seal in the late stages of hydrolysis. Above: Fluorocarbon (FPM) seal showing early signs of hydrolysis. Above: Fluorocarbon (FPM) seal showing late stages of hydrolysis. Swelling Fluid media absorbed into an incompatible seal material causes the material to deform, and swell. Discoloration may be associated with swelling as well. CONTRIBUTING FACTORS Incompatible seal material for fluid used High temperatures Above: Swelling failure of a dirt wiper. Wiper at top is new for comparison. 014 015 systemseals.com
- 9. Side Loading Damage to the sealing components during extreme side loads that exceed the guidance capability. Result is usually metal-to-metal contact with severe damage to all components CONTRIBUTING FACTORS Insufficient guidance High temperatures, which can degrade certain types of guide bushing materials Ineffective placement of the bushings within the cylinder Above: Severe side loading with catastrophic damage from metal-to-metal contact. Above: Side loading that wore the chrome off the rod. Flex Fatigue/ Fracturing The deformation of the seal under pressure creates tensile stresses that can fatigue and fracture the seal material. CONTRIBUTING FACTORS Incorrect seal design High pressures High cycle rate Short cycle time Above: Opposing tensile stresses flex the seal material during each pressure cycle, fatiguing the material over time. The stresses fatigue the material to the breaking point. Above: Front view of a polyurethane seal with a flex fatigue crack through the middle section of the seal. Above: Profile section of an o-ring loaded u-cup with flex fatigue cracking. 016 017 systemseals.com
- 10. Above: Section profile of the above seal showing wear and loss of pre-load. Note the dynamic lip (bottom lip) has lost its sharp edge and h